#------------------------------------------------------------------------------
#$Date: 2016-02-19 16:29:56 +0200 (Fri, 19 Feb 2016) $
#$Revision: 176759 $
#$URL: svn://www.crystallography.net/cod/cif/2/00/40/2004007.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2004007
loop_
_publ_author_name
'Britten, J. F.'
'Dabkowska, H. A.'
'Dabkowski, A. B.'
'Greedan, J. E.'
'Campbell, J. L.'
'Teesdale, W. J.'
_publ_section_title
;
 Czochralski-Grown SrLaGaO₄
;
_journal_issue                   10
_journal_name_full               'Acta Crystallographica Section C'
_journal_page_first              1975
_journal_page_last               1977
_journal_paper_doi               10.1107/S0108270194011820
_journal_volume                  51
_journal_year                    1995
_chemical_formula_analytical     'Ga La O4 Sr'
_chemical_formula_structural     'Ga La O4 Sr'
_chemical_formula_sum            'Ga La O4 Sr'
_chemical_formula_weight         360.25
_chemical_melting_point          1793
_chemical_name_common            'strontium lanthanum gallate'
_chemical_name_systematic
;
 strontium lanthanum gallate
;
_space_group_IT_number           139
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_audit_creation_method           SHELXL
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   3.8437(3)
_cell_length_b                   3.8437(3)
_cell_length_c                   12.6880(15)
_cell_measurement_reflns_used    23
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      110.1
_cell_measurement_theta_min      87.3
_cell_measurement_wavelength     .55941
_cell_volume                     187.45(3)
_computing_cell_refinement
' R3m/V Crystallographic Research System using Kα₁ (Siemens, 1989)'
_computing_data_collection
' R3m/V Crystallographic Research System using Kα₁ (Siemens, 1989)'
_computing_data_reduction
' R3m/V Crystallographic Research System (Siemens, 1989)'
_computing_molecular_graphics    'SHELXTL/PC (Sheldrick, 1992)'
_computing_publication_material  'SHELXL93 (Sheldrick, 1994)'
_computing_structure_refinement  'SHELXL93 (Sheldrick, 1994)'
_computing_structure_solution
' TEXSAN (Molecular Structure Corporation, 1992)'
_diffrn_ambient_temperature      296(2)
_diffrn_measurement_device       'Siemens R3m/V'
_diffrn_measurement_method       2θ-θ
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           AgK\a
_diffrn_radiation_wavelength     .56086
_diffrn_reflns_av_R_equivalents  .0281
_diffrn_reflns_av_sigmaI/netI    0.0311
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       37
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            1868
_diffrn_reflns_theta_max         55.29
_diffrn_reflns_theta_min         2.53
_diffrn_standards_decay_%        .00
_diffrn_standards_interval_count 97
_diffrn_standards_number         3
_exptl_absorpt_coefficient_mu    17.255
_exptl_absorpt_correction_T_max  .10408
_exptl_absorpt_correction_T_min  .03751
_exptl_absorpt_correction_type   sphere
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    6.383
_exptl_crystal_density_meas      6.388(9)
_exptl_crystal_density_method    displacement
_exptl_crystal_description       'ground sphere'
_exptl_crystal_F_000             316
_exptl_crystal_size_rad          .152(4)
_refine_diff_density_max         4.982
_refine_diff_density_min         -03.994
_refine_ls_extinction_coef       .132(6)
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_all   1.156
_refine_ls_goodness_of_fit_obs   1.187
_refine_ls_matrix_type           full
_refine_ls_number_parameters     13
_refine_ls_number_reflns         780
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.157
_refine_ls_restrained_S_obs      1.187
_refine_ls_R_factor_all          0.0324
_refine_ls_R_factor_obs          .0272
_refine_ls_shift/esd_max         .001
_refine_ls_shift/esd_mean        0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_scheme
;
w = 1/[\s^2^(F~o~^2^) + (0.0317P)^2^ + 0.2075P]
where P = (F~o~^2^ + 2F~c~^2^)/3
;
_refine_ls_wR_factor_all         .0679
_refine_ls_wR_factor_obs         .0662
_reflns_number_observed          706
_reflns_number_total             781
_reflns_observed_criterion       >2\s~I~
_cod_data_source_file            jz1003.cif
_cod_data_source_block           SrLaGaO~4~
_cod_depositor_comments
;
The following automatic conversions were performed:

'_geom_bond_publ_flag' value 'Y' changed to 'y' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (5
times).

'_geom_angle_publ_flag' value 'Y' changed to 'y' according
to /home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary
named 'cif_core.dic' version 2.4.1 from 2010-06-29 (15 times).

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_cell_volume        188.45(3)
_cod_database_code               2004007
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-y, x, z'
'y, -x, z'
'-x, y, -z'
'x, -y, -z'
'y, x, -z'
'-y, -x, -z'
'x+1/2, y+1/2, z+1/2'
'-x+1/2, -y+1/2, z+1/2'
'-y+1/2, x+1/2, z+1/2'
'y+1/2, -x+1/2, z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'y+1/2, x+1/2, -z+1/2'
'-y+1/2, -x+1/2, -z+1/2'
'-x, -y, -z'
'x, y, -z'
'y, -x, -z'
'-y, x, -z'
'x, -y, z'
'-x, y, z'
'-y, -x, z'
'y, x, z'
'-x+1/2, -y+1/2, -z+1/2'
'x+1/2, y+1/2, -z+1/2'
'y+1/2, -x+1/2, -z+1/2'
'-y+1/2, x+1/2, -z+1/2'
'x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, z+1/2'
'-y+1/2, -x+1/2, z+1/2'
'y+1/2, x+1/2, z+1/2'
loop_
_atom_site_label
_atom_site_occupancy
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_thermal_displace_type
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_type_symbol
La .50 0 0 .358673(14) .00557(4) Uani d SP La
Sr .50 0 0 .358673(14) .00557(4) Uani d SP Sr
Ga 1 0 0 0 .00710(6) Uani d S Ga
O1 1 0 0 .1673(2) .0144(5) Uani d S O
O2 1 0 .5 0 .0072(2) Uani d S O
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_source
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
O O 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' .0056 .0036
Ga Ga 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' .3179 1.0589
Sr Sr 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' -0.1172 2.2025
La La 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' -0.6411 1.6148
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
O1 La O2 . 11 133.016(5) y
O1 La O2 . 9_545 133.016(5) ?
O2 La O2 11 9_545 62.264(6) y
O1 La O2 . 11_545 133.016(5) y
O2 La O2 11 11_545 93.968(10) y
O2 La O2 9_545 11_545 62.264(5) ?
O1 La O2 . 9_445 133.016(5) ?
O2 La O2 11 9_445 62.264(5) ?
O2 La O2 9_545 9_445 93.968(10) ?
O2 La O2 11_545 9_445 62.264(6) ?
O1 La O1 . 25_445 83.09(6) y
O2 La O1 11 25_445 126.53(5) y
O2 La O1 9_545 25_445 126.53(5) ?
O2 La O1 11_545 25_445 64.46(5) y
O2 La O1 9_445 25_445 64.46(5) ?
O1 La O1 . 25 83.09(6) ?
O2 La O1 11 25 64.46(5) ?
O2 La O1 9_545 25 64.46(5) ?
O2 La O1 11_545 25 126.53(5) ?
O2 La O1 9_445 25 126.53(5) ?
O1 La O1 25_445 25 166.18(12) y
O1 La O1 . 25_455 83.09(6) ?
O2 La O1 11 25_455 64.46(5) ?
O2 La O1 9_545 25_455 126.53(5) ?
O2 La O1 11_545 25_455 126.53(5) ?
O2 La O1 9_445 25_455 64.46(5) ?
O1 La O1 25_445 25_455 89.171(14) y
O1 La O1 25 25_455 89.171(14) ?
O1 La O1 . 25_545 83.09(6) ?
O2 La O1 11 25_545 126.53(5) ?
O2 La O1 9_545 25_545 64.46(5) ?
O2 La O1 11_545 25_545 64.46(5) ?
O2 La O1 9_445 25_545 126.53(5) ?
O1 La O1 25_445 25_545 89.171(14) ?
O1 La O1 25 25_545 89.171(14) ?
O1 La O1 25_455 25_545 166.18(12) ?
O1 La Ga . 9 123.415(5) ?
O2 La Ga 11 9 36.173(2) ?
O2 La Ga 9_545 9 36.173(2) ?
O2 La Ga 11_545 9 93.202(8) ?
O2 La Ga 9_445 9 93.202(8) ?
O1 La Ga 25_445 9 153.49(6) ?
O1 La Ga 25 9 40.32(6) ?
O1 La Ga 25_455 9 93.80(3) ?
O1 La Ga 25_545 9 93.80(3) ?
O1 La Ga . 9_455 123.415(5) ?
O2 La Ga 11 9_455 36.173(2) ?
O2 La Ga 9_545 9_455 93.202(8) ?
O2 La Ga 11_545 9_455 93.202(8) ?
O2 La Ga 9_445 9_455 36.173(2) ?
O1 La Ga 25_445 9_455 93.80(3) ?
O1 La Ga 25 9_455 93.80(3) ?
O1 La Ga 25_455 9_455 40.32(6) ?
O1 La Ga 25_545 9_455 153.49(6) ?
Ga La Ga 9 9_455 72.346(4) ?
O1 La Ga . 9_545 123.415(5) ?
O2 La Ga 11 9_545 93.202(8) ?
O2 La Ga 9_545 9_545 36.173(2) ?
O2 La Ga 11_545 9_545 36.173(2) ?
O2 La Ga 9_445 9_545 93.202(8) ?
O1 La Ga 25_445 9_545 93.80(3) ?
O1 La Ga 25 9_545 93.80(3) ?
O1 La Ga 25_455 9_545 153.49(6) ?
O1 La Ga 25_545 9_545 40.32(6) ?
Ga La Ga 9 9_545 72.346(4) ?
Ga La Ga 9_455 9_545 113.170(9) ?
O1 Sr O2 . 11 133.016(5) ?
O1 Sr O2 . 9_545 133.016(5) ?
O2 Sr O2 11 9_545 62.264(6) ?
O1 Sr O2 . 11_545 133.016(5) ?
O2 Sr O2 11 11_545 93.968(10) ?
O2 Sr O2 9_545 11_545 62.264(5) ?
O1 Sr O2 . 9_445 133.016(5) ?
O2 Sr O2 11 9_445 62.264(5) ?
O2 Sr O2 9_545 9_445 93.968(10) ?
O2 Sr O2 11_545 9_445 62.264(6) ?
O1 Sr O1 . 25_445 83.09(6) ?
O2 Sr O1 11 25_445 126.53(5) ?
O2 Sr O1 9_545 25_445 126.53(5) ?
O2 Sr O1 11_545 25_445 64.46(5) ?
O2 Sr O1 9_445 25_445 64.46(5) ?
O1 Sr O1 . 25 83.09(6) ?
O2 Sr O1 11 25 64.46(5) ?
O2 Sr O1 9_545 25 64.46(5) ?
O2 Sr O1 11_545 25 126.53(5) ?
O2 Sr O1 9_445 25 126.53(5) ?
O1 Sr O1 25_445 25 166.18(12) ?
O1 Sr O1 . 25_455 83.09(6) ?
O2 Sr O1 11 25_455 64.46(5) ?
O2 Sr O1 9_545 25_455 126.53(5) ?
O2 Sr O1 11_545 25_455 126.53(5) ?
O2 Sr O1 9_445 25_455 64.46(5) ?
O1 Sr O1 25_445 25_455 89.171(14) ?
O1 Sr O1 25 25_455 89.171(14) ?
O1 Sr O1 . 25_545 83.09(6) ?
O2 Sr O1 11 25_545 126.53(5) ?
O2 Sr O1 9_545 25_545 64.46(5) ?
O2 Sr O1 11_545 25_545 64.46(5) ?
O2 Sr O1 9_445 25_545 126.53(5) ?
O1 Sr O1 25_445 25_545 89.171(14) ?
O1 Sr O1 25 25_545 89.171(14) ?
O1 Sr O1 25_455 25_545 166.18(12) ?
O1 Sr Ga . 9 123.415(5) ?
O2 Sr Ga 11 9 36.173(2) ?
O2 Sr Ga 9_545 9 36.173(2) ?
O2 Sr Ga 11_545 9 93.202(8) ?
O2 Sr Ga 9_445 9 93.202(8) ?
O1 Sr Ga 25_445 9 153.49(6) ?
O1 Sr Ga 25 9 40.32(6) ?
O1 Sr Ga 25_455 9 93.80(3) ?
O1 Sr Ga 25_545 9 93.80(3) ?
O1 Sr Ga . 9_455 123.415(5) ?
O2 Sr Ga 11 9_455 36.173(2) ?
O2 Sr Ga 9_545 9_455 93.202(8) ?
O2 Sr Ga 11_545 9_455 93.202(8) ?
O2 Sr Ga 9_445 9_455 36.173(2) ?
O1 Sr Ga 25_445 9_455 93.80(3) ?
O1 Sr Ga 25 9_455 93.80(3) ?
O1 Sr Ga 25_455 9_455 40.32(6) ?
O1 Sr Ga 25_545 9_455 153.49(6) ?
Ga Sr Ga 9 9_455 72.346(4) ?
O1 Sr Ga . 9_545 123.415(5) ?
O2 Sr Ga 11 9_545 93.202(8) ?
O2 Sr Ga 9_545 9_545 36.173(2) ?
O2 Sr Ga 11_545 9_545 36.173(2) ?
O2 Sr Ga 9_445 9_545 93.202(8) ?
O1 Sr Ga 25_445 9_545 93.80(3) ?
O1 Sr Ga 25 9_545 93.80(3) ?
O1 Sr Ga 25_455 9_545 153.49(6) ?
O1 Sr Ga 25_545 9_545 40.32(6) ?
Ga Sr Ga 9 9_545 72.346(4) ?
Ga Sr Ga 9_455 9_545 113.170(9) ?
O2 Ga O2 3_655 3 180.0 ?
O2 Ga O2 3_655 . 90.0 ?
O2 Ga O2 3 . 90.0 ?
O2 Ga O2 3_655 1_545 90.0 ?
O2 Ga O2 3 1_545 90.0 ?
O2 Ga O2 . 1_545 180.0 ?
O2 Ga O1 3_655 17 90.0 ?
O2 Ga O1 3 17 90.0 ?
O2 Ga O1 . 17 90.0 ?
O2 Ga O1 1_545 17 90.0 ?
O2 Ga O1 3_655 . 90.0 ?
O2 Ga O1 3 . 90.0 ?
O2 Ga O1 . . 90.0 ?
O2 Ga O1 1_545 . 90.0 ?
O1 Ga O1 17 . 180.0 ?
O2 Ga La 3_655 9_444 126.173(2) ?
O2 Ga La 3 9_444 53.827(2) ?
O2 Ga La . 9_444 126.173(2) ?
O2 Ga La 1_545 9_444 53.827(2) ?
O1 Ga La 17 9_444 56.585(5) ?
O1 Ga La . 9_444 123.415(5) ?
O2 Ga Sr 3_655 25 53.827(2) ?
O2 Ga Sr 3 25 126.173(2) ?
O2 Ga Sr . 25 53.827(2) ?
O2 Ga Sr 1_545 25 126.173(2) ?
O1 Ga Sr 17 25 123.415(5) ?
O1 Ga Sr . 25 56.585(5) ?
La Ga Sr 9_444 25 180.0 ?
O2 Ga Sr 3_655 9_444 126.173(2) ?
O2 Ga Sr 3 9_444 53.827(2) ?
O2 Ga Sr . 9_444 126.173(2) ?
O2 Ga Sr 1_545 9_444 53.827(2) ?
O1 Ga Sr 17 9_444 56.585(5) ?
O1 Ga Sr . 9_444 123.415(5) ?
La Ga Sr 9_444 9_444 0.000(5) ?
Sr Ga Sr 25 9_444 180.0 ?
O2 Ga La 3_655 25 53.827(2) ?
O2 Ga La 3 25 126.173(2) ?
O2 Ga La . 25 53.827(2) ?
O2 Ga La 1_545 25 126.173(2) ?
O1 Ga La 17 25 123.415(5) ?
O1 Ga La . 25 56.585(5) ?
La Ga La 9_444 25 180.0 ?
Sr Ga La 25 25 0.000(5) ?
Sr Ga La 9_444 25 180.0 ?
O2 Ga La 3_655 9_554 53.827(2) ?
O2 Ga La 3 9_554 126.173(2) ?
O2 Ga La . 9_554 53.827(2) ?
O2 Ga La 1_545 9_554 126.173(2) ?
O1 Ga La 17 9_554 56.585(5) ?
O1 Ga La . 9_554 123.415(5) ?
La Ga La 9_444 9_554 113.170(9) ?
Sr Ga La 25 9_554 66.830(9) ?
Sr Ga La 9_444 9_554 113.170(9) ?
La Ga La 25 9_554 66.830(9) ?
O2 Ga La 3_655 25_445 126.173(2) ?
O2 Ga La 3 25_445 53.827(2) ?
O2 Ga La . 25_445 126.173(2) ?
O2 Ga La 1_545 25_445 53.827(2) ?
O1 Ga La 17 25_445 123.415(5) ?
O1 Ga La . 25_445 56.585(5) ?
La Ga La 9_444 25_445 66.830(9) ?
Sr Ga La 25 25_445 113.170(9) ?
Sr Ga La 9_444 25_445 66.830(9) ?
La Ga La 25 25_445 113.170(9) ?
La Ga La 9_554 25_445 180.0 ?
Ga O1 La . . 180.0 ?
Ga O1 Sr . . 180.0 ?
La O1 Sr . . 0.0 ?
Ga O1 Sr . 25_445 83.09(6) ?
La O1 Sr . 25_445 96.91(6) ?
Sr O1 Sr . 25_445 96.91(6) ?
Ga O1 La . 25_445 83.09(6) y
La O1 La . 25_445 96.91(6) y
Sr O1 La . 25_445 96.91(6) ?
Sr O1 La 25_445 25_445 0.000(7) ?
Ga O1 Sr . 25 83.09(6) ?
La O1 Sr . 25 96.91(6) ?
Sr O1 Sr . 25 96.91(6) ?
Sr O1 Sr 25_445 25 166.18(12) ?
La O1 Sr 25_445 25 166.18(12) ?
Ga O1 La . 25 83.09(6) ?
La O1 La . 25 96.91(6) ?
Sr O1 La . 25 96.91(6) ?
Sr O1 La 25_445 25 166.18(12) ?
La O1 La 25_445 25 166.18(12) y
Sr O1 La 25 25 0.000(7) ?
Ga O1 La . 25_455 83.09(6) ?
La O1 La . 25_455 96.91(6) ?
Sr O1 La . 25_455 96.91(6) ?
Sr O1 La 25_445 25_455 89.171(14) ?
La O1 La 25_445 25_455 89.171(14) y
Sr O1 La 25 25_455 89.171(14) ?
La O1 La 25 25_455 89.171(14) ?
Ga O1 La . 25_545 83.09(6) ?
La O1 La . 25_545 96.91(6) ?
Sr O1 La . 25_545 96.91(6) ?
Sr O1 La 25_445 25_545 89.171(14) ?
La O1 La 25_445 25_545 89.171(14) ?
Sr O1 La 25 25_545 89.171(14) ?
La O1 La 25 25_545 89.171(14) ?
La O1 La 25_455 25_545 166.18(12) ?
Ga O1 Sr . 25_545 83.09(6) ?
La O1 Sr . 25_545 96.91(6) ?
Sr O1 Sr . 25_545 96.91(6) ?
Sr O1 Sr 25_445 25_545 89.171(14) ?
La O1 Sr 25_445 25_545 89.171(14) ?
Sr O1 Sr 25 25_545 89.171(14) ?
La O1 Sr 25 25_545 89.171(14) ?
La O1 Sr 25_455 25_545 166.18(12) ?
La O1 Sr 25_545 25_545 0.000(7) ?
Ga O1 Sr . 25_455 83.09(6) ?
La O1 Sr . 25_455 96.91(6) ?
Sr O1 Sr . 25_455 96.91(6) ?
Sr O1 Sr 25_445 25_455 89.171(14) ?
La O1 Sr 25_445 25_455 89.171(14) ?
Sr O1 Sr 25 25_455 89.171(14) ?
La O1 Sr 25 25_455 89.171(14) ?
La O1 Sr 25_455 25_455 0.000(7) ?
La O1 Sr 25_545 25_455 166.18(12) ?
Sr O1 Sr 25_545 25_455 166.18(12) ?
Ga O2 Ga 1_565 . 180.0 ?
Ga O2 La 1_565 9_454 90.0 ?
Ga O2 La . 9_454 90.0 ?
Ga O2 Sr 1_565 25 90.0 ?
Ga O2 Sr . 25 90.0 ?
La O2 Sr 9_454 25 180.0 ?
Ga O2 Sr 1_565 9_454 90.0 ?
Ga O2 Sr . 9_454 90.0 ?
La O2 Sr 9_454 9_454 0.000(6) ?
Sr O2 Sr 25 9_454 180.0 ?
Ga O2 La 1_565 25 90.0 ?
Ga O2 La . 25 90.0 ?
La O2 La 9_454 25 180.0 ?
Sr O2 La 25 25 0.000(6) ?
Sr O2 La 9_454 25 180.0 ?
Ga O2 La 1_565 9_554 90.0 ?
Ga O2 La . 9_554 90.0 ?
La O2 La 9_454 9_554 93.968(10) y
Sr O2 La 25 9_554 86.032(10) ?
Sr O2 La 9_454 9_554 93.968(10) ?
La O2 La 25 9_554 86.032(10) y
Ga O2 Sr 1_565 9_554 90.0 ?
Ga O2 Sr . 9_554 90.0 ?
La O2 Sr 9_454 9_554 93.968(10) ?
Sr O2 Sr 25 9_554 86.032(10) ?
Sr O2 Sr 9_454 9_554 93.968(10) ?
La O2 Sr 25 9_554 86.032(10) ?
La O2 Sr 9_554 9_554 0.000(6) ?
Ga O2 Sr 1_565 25_455 90.0 ?
Ga O2 Sr . 25_455 90.0 ?
La O2 Sr 9_454 25_455 86.032(10) ?
Sr O2 Sr 25 25_455 93.968(10) ?
Sr O2 Sr 9_454 25_455 86.032(10) ?
La O2 Sr 25 25_455 93.968(10) ?
La O2 Sr 9_554 25_455 180.0 ?
Sr O2 Sr 9_554 25_455 180.0 ?
Ga O2 La 1_565 25_455 90.0 ?
Ga O2 La . 25_455 90.0 ?
La O2 La 9_454 25_455 86.032(10) ?
Sr O2 La 25 25_455 93.968(10) ?
Sr O2 La 9_454 25_455 86.032(10) ?
La O2 La 25 25_455 93.968(10) ?
La O2 La 9_554 25_455 180.0 ?
Sr O2 La 9_554 25_455 180.0 ?
Sr O2 La 25_455 25_455 0.000(6) ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
La O1 . 2.428(3) y
La O2 11 2.6285(2) y
La O2 9_545 2.6285(2) ?
La O2 11_545 2.6285(2) ?
La O2 9_445 2.6285(2) ?
La O1 25_445 2.7378(4) y
La O1 25 2.7378(4) ?
La O1 25_455 2.7378(4) ?
La O1 25_545 2.7378(4) ?
La Ga 9 3.2561(2) ?
La Ga 9_455 3.2561(2) ?
La Ga 9_545 3.2561(2) ?
Sr O1 . 2.428(3) ?
Sr O2 11 2.6285(2) ?
Sr O2 9_545 2.6285(2) ?
Sr O2 11_545 2.6285(2) ?
Sr O2 9_445 2.6285(2) ?
Sr O1 25_445 2.7378(4) ?
Sr O1 25 2.7378(4) ?
Sr O1 25_455 2.7378(4) ?
Sr O1 25_545 2.7378(4) ?
Sr Ga 9 3.2561(2) ?
Sr Ga 9_455 3.2561(2) ?
Sr Ga 9_545 3.2561(2) ?
Ga O2 3_655 1.9218(2) ?
Ga O2 3 1.9218(2) ?
Ga O2 . 1.9218(2) y
Ga O2 1_545 1.9218(2) ?
Ga O1 17 2.122(3) ?
Ga O1 . 2.122(3) y
Ga La 9_444 3.2561(2) ?
Ga Sr 25 3.2561(2) ?
Ga Sr 9_444 3.2561(2) ?
Ga La 25 3.2561(2) ?
Ga La 9_554 3.2561(2) ?
Ga La 25_445 3.2561(2) ?
O1 Sr 25_445 2.7378(4) ?
O1 La 25_445 2.7378(4) ?
O1 Sr 25 2.7378(4) ?
O1 La 25 2.7378(4) ?
O1 La 25_455 2.7378(4) ?
O1 La 25_545 2.7378(4) ?
O1 Sr 25_545 2.7378(4) ?
O1 Sr 25_455 2.7378(4) ?
O2 Ga 1_565 1.9218(2) ?
O2 La 9_454 2.6285(2) ?
O2 Sr 25 2.6285(2) ?
O2 Sr 9_454 2.6285(2) ?
O2 La 25 2.6285(2) ?
O2 La 9_554 2.6285(2) ?
O2 Sr 9_554 2.6285(2) ?
O2 Sr 25_455 2.6285(2) ?
O2 La 25_455 2.6285(2) ?
